Natural blue zircon from VesuviusBlue colouration in Vesuvius zircon is explained by the effect of...
Embed Size (px)
Transcript of Natural blue zircon from VesuviusBlue colouration in Vesuvius zircon is explained by the effect of...
Natural blue zircon from Vesuvius
Yi Sun1,2 & Axel K. Schmitt1 & Tobias Häger3 & Marcus Schneider1 & Lucia Pappalardo4 & Massimo Russo4
Received: 31 March 2020 /Accepted: 15 October 2020# The Author(s) 2020
AbstractZircon from syenitic ejecta of Vesuvius (Campania, Italy) is unusually blue, a property shared with gem zircon fromRatanakiri province (Cambodia), which turns from natural reddish-brown to blue when heated under reducing conditions.Here, the origins of these unusual crystals were traced through geochronology, trace elements, and O-Hf isotopic compo-sitions. The causes of its colour were investigated through optical and electron microscopy, optical absorption spectroscopy,and Raman microspectroscopy. Colour stability upon heating and ultraviolet light (UV) exposure was tested usingRatanakiri zircon as a control. Vesuvius zircon contains vesiculated zones with abundant inclusions ~2.5 μm to 15 h). Turbid domains rich in large inclusions change to yellow-brown after heating underoxidizing conditions, while transparent domains remain pale blue or colourless. Optical absorption spectra display sharpabsorption lines attributed to U4+, and slightly elevated absorption towards shorter wavelengths. The ~1007 cm−1 ν3(SiO4)Raman band is broadened due to lattice distortion by non-stoichiometric elements in high-Th/-U zircon, whereas narrowbands in inclusion-rich domains indicate a decrease in lattice strain due to inclusion precipitation. Blue colouration inVesuvius zircon is explained by the effect of light scattering (Rayleigh and/or Mie scattering) on highly refractiveactinide-rich inclusions ranging in size from
Commercially marketed blue coloured gem zircon is gen-erally artificially produced by heat-treatment of reddish-brown natural zircon crystals (Fig. 1 a) at temperatures of~1000 °C under reducing conditions for several hours (e.g.,Satitkune et al. 2013; Wittwer et al. 2013; Zeug et al. 2018).Dark red-brown zircon crystals from the Bei Srok area(Ratanakiri province, Cambodia) are specifically susceptibleto this colour change (Piilonen et al. 2018), although lessintense blue colouration can also be achieved using raw ma-terial from other mines in Ratanakiri province (Piilonen et al.2018) as well as from Chanthaburi and Kanchanaburi(Thailand; Satitkune et al. 2013; Zeug et al. 2018); ShanState (Myanmar; Zeug et al. 2018) or the Central Highlands(Vietnam; Huong et al. 2016). Also, the colour of dark greenmetamict zircon from Ratnapura (Sri Lanka) can be thermallyenhanced to light blue by heat treatment under similar condi-tions (Rupasinghe and Senaratne 1986).
At present, there is no theory which can fully explain both(1) the colour change to blue induced by heating under
reduced conditions and (2) the special susceptibility ofRatanakiri brown zircon for this phenomenon (Zeug et al.2018). While the presence of a broad absorption band centredat ~640 nmwas shown to be responsible for the blue colour ofheated Ratanakiri zircon by optical spectroscopy, its attribu-tion to a specific chromophore (e.g., U4+, Tb3+) is still prob-lematic and controversially discussed (Zeug et al. 2018).Understanding the causes of blue colouration in zircon is ofimportance for optimization of the heat-treatment techniqueused and can help to improve the qualitative output of theseheat-treated gemstones.
Blue zircon of unambiguously natural origin has only beenreported for one occurrence: volcanic ejecta from the westernflank of Vesuvius volcano (Campania, Italy; Russo and Punzo2004; Kempe et al. 2016; Zeug et al. 2018). Kempe et al.(2016) suggested that reheating of early-formed zircon crys-tals by ascending magma during eruption might be responsi-ble for the blue colour; thus Vesuvius blue zircon (Fig. 1 b;Fig. S1-S2 in the electronic supplementary material (ESM))might represent a natural analogue for heat-treated Ratanakiri-type gem zircon. Insufficient sample dimensions, however,prevented the acquisition of optical spectra (Kempe et al.2016), and no further mineralogical characterization ofVesuvius blue zircon has been published yet. Here, we presentthe first comprehensive characterization of Vesuvius blue zir-con (including quantitative chemical analysis of trace ele-ments and O-Hf isotopes, geochronology, optical and electronmicroscopy, as well as optical absorption spectroscopy andRaman microspectroscopy) to determine the origin of theseunusual crystals, while also proposing a previously undocu-mented mechanism for the blue colour of Vesuvius zircon thatdiffers from that of heat-treated Ratanakiri zircon.
The Bronze Age Avellino pumice eruption (3945 ± 10 cal BP;Sevink et al. 2011) represents one of the four major Plinianeruptions of Monte Somma-Vesuvius (Campania, Italy) dur-ing the last 22 ka BP (e.g., Di Renzo et al. 2007; Santacroceet al. 2008). The vent area of the Avellino pumice eruptionwas located at the Piano della Gianestre, and proximal pyro-clastic fall deposits were deposited at the western flank ofSomma-Vesuvius (Cioni et al. 1999; Linde et al. 2017).Accessory lithic ejecta, including nodules of subvolcanic sy-enite, cumulate rocks (e.g., pyroxenite) and skarns, are abun-dant in the central to upper stratigraphic units of the pyroclas-tic sequence (EU3-EU5; Sulpizio et al. 2010a, 2010b).
The syenitic ejecta originated from the crystalline carapaceof the magma reservoir where they crystallized from highlyfractionated melts or fluids in the uppermost, most evolvedsections of the magma chamber (e.g., Fulignati et al. 2004).Magmatic temperatures are estimated as ~1200 °C for the
Fig. 1 Focus-stacked optical images of blue zircon crystals: a) heat-treated blue zircon as a cut gemstone likely from Ratanakiri; b) naturalblue Vesuvius zircon crystal growing in interstitial volumes betweensanidine crystals, collected from the San Vito Quarry near Ercolano
22 Y. Sun et al.
tephritic source magma, and ~ 800 °C for the highly evolved,phonolitic melts erupted during the Avellino eruption (Barberiet al. 1981; Balcone-Boissard et al. 2012). Extremely highzircon saturation levels (~12,000 ppm) are expected for themafic, tephritic source melts of Vesuvius considering the con-ditions in the magma chamber (T = 1200 °C; P = 0.2 GPa;Balcone-Boissard et al. 2012) and equations by Shao et al.(2019), reinforcing a propensity for zircon to crystallize fromtheir more felsic differentiates. Slightly oxidized magma con-ditions with oxygen fugacity (fO2) of +1.24 above the Ni-NiObuffer (NNO) were calculated for Avellino phonolite usingstable sulphur isotope ratios (Marini et al. 1998).
Materials and methods
Sample material and thin-section petrography
Two zircon-bearing syenite clasts were collected from the SanVito Quarry, Ercolano (40 °49′50.91´´N – 14 °22′54.84″E).Themedium to coarse-grained syenite is porous (pore volume~ 10–30%) with a granular isotropic texture and contains as amajor constituent lath-shaped and idiomorphic sanidine crys-tals (Fig. 2 a) up to 2 mm length, often with Carlsbad twin-ning. Sodalite occurs as poikilitic crystals along with opaqueFe-Ti oxides and biotite forming subhedral crystals up to2 mm in size (Fig. 2 a). Accessory apatite, fluorite, and mem-bers of the pyrochlore group are present as minute (
and spectroscopy. These crystals were mounted in epoxy,ground to a uniform thickness between ~200 μm and400 μm (depending on crystal size), and polished on bothsides. Samples were then removed from the epoxy resin; foreasier handling, zircon chips were attached to 2.5 mm copperrings using a thermoplastic adhesive. After obtaining opticalabsorption spectra, the adhesive was dissolved in ethanol andthe zircon chips were mounted in epoxy (Erc-z2) for furthercharacterization.
Heating and UV irradiation experiments
Vesuvius and Ratanakiri zircon grains were heat-treated tocompare their colour changes during thermal annealing atvarying fO2. The colour stability of the zircon grains underultraviolet (UV) irradiation was then tested on both heat-treated and natural zircon grains. A vertical CO2/CO gasmixing furnace by Gero Hochtemperaturöfen GmbH wasused for experiments under reduced conditions. The furnacewas held at a constant temperature of 1000 °C during thecourse of the experiments, considering 900–1000 °C as thetypical temperature range for commercial heat-treatment ofgem zircon as reported in the literature (e.g., Wittwer et al.2013; Zeug et al. 2018). Zircon grains were placed on a plat-inum mesh and introduced into the pre-heated furnace. As theexact method for thermal colour enhancement remains secretand further information about the fO2 conditions used wereunavailable (e.g., Zeug et al. 2018), experiments were run atvarying fO2 levels maintained by adjusting the CO2:COmixing ratio (Air Liquide carbon dioxide 4.5, UN 1013; AirLiquide carbon monoxide 3.7, UN 1016) in the furnace. Thefollowing mixing ratios were used during the experiments: (1)CO2:CO = 60:40 vol%; (2) CO2:CO = 80:20 vol%, corre-sponding to fO2 near the IW (iron-wüstite) buffer; (3) pureCO, representing the lowest fO2 achievable using CO-basedgas mixing furnaces. Prior to sample removal, the furnace wasflooded with pure CO2 for about one minute to prevent theemission of CO. As quenching in cold water could potentiallydestroy the zircon crystals, samples were directly releasedfrom the 1000 °C hot furnace onto a ceramic plate and imme-diately transferred into a porcelain crucible for cooling. After aseries of initial experiments, single crystals of Vesuvius bluezircon and brown Ratanakiri zircon were heated together in apure CO atmosphere at 1000 °C for 18 h. Heat-treating underoxidizing conditions was carried out in a box furnace, wherezircon grains were placed in a platinum crucible and heated for24 h at 1000 °C in ambient atmosphere.
The stability of blue zircon colouration under UV light wasexperimentally tested for both Vesuvius and Ratanakiri sam-ples, as colour changes of blue gem zircons to light brownunder the influence of long-wave UV light have been de-scribed before (Renfro 2016). For this purpose, heat-treatedRatanakiri samples and untreated Vesuvius blue zircon were
irradiated under both short-wave (254 nm) and long-wave(365 nm) UV light for ca. 1 h each using a Vilber LourmatVL-4.LC with 4 W lamps.
A Zeiss Stemi 508 stereo microscope with an attachedAxioCam ICc1 camera was used to image doubly-polishedzircon chips immersed in mineral oil using transmitted anddarkfield illumination. Comparison of the colour appearancein both illuminations is a test for scattering, as long-wavelength light is scattered less than short-wavelength light,leading to a brownish-reddish tint in transmitted light, and ablueish colour in darkfield illumination (e.g., Pelto 1956).This was verified by imaging a fragment of commerciallyavailable synthetic cryolite glass (aka opal glass) under thesame conditions, where the variable colour appearance is at-tributed to light scattering by sub-μm Ca- and Na-fluorideparticles (Ryde and Cooper 1931). A similar test was per-formed on a piece of blue chalcedony (Fig. S3 in the ESM),another material where blue colouration has been suspected asbeing due to scattering (Pelto 1956).
Scanning electron microscopy (SEM) andmicrotomography (micro-CT)
Epoxy mounts were conductively coated with 3 nm gold andimaged with a Zeiss EVO MA15 scanning electron micro-scope equipped with a Gatan ChromaCL2 detector forcathodoluminescence (CL) imaging. Back-scattered electron(BSE) and CL images were obtained from zircon to reveal itsinternal structure, including growth zones and inclusions. Forsemi-quantitative elemental analysis using energy dispersiveX-ray spectroscopy (EDS) the epoxy mounts were recoatedwith carbon and analyzed with an Oxford Instruments X-MaxN 150 mm2 EDS detector on the same instrument.Additional imaging and elemental analysis of heat-treatedVesuvius zircon crystals were performed using a Zeiss Leo440 instrument equipped with an Oxford Instruments X-Max80 mm2 EDS detector.
The textural arrangement of inclusions in Vesuvius bluezircon was also visualized using computed microtomography(micro-CT) X-ray analysis using a Carl Zeiss Xradia Versa-410 3D X-ray microscope. The instrument was operated witha polychromatic microfocus X-ray source (150 kV, 10 W), a2000 × 2000 pixel noise-suppressed charge-coupled detector,and a 10× objective lens to achieve a resolution of 1.88 μm/voxel. 3201 projections over 360 ° were generated for themeasurement. Attenuation data were reconstructed through afiltered back-projection algorithm using the XRMRe con-structor software, producing a stack of 967 cross-sectional,grey-scale digital images that are displayed in animation style(see Animation S1 in the ESM).
24 Y. Sun et al.
Secondary ionization mass spectrometry (SIMS) andlaser ablation inductively coupled plasma mass spec-trometry (LA-ICP-MS) analysis
Prior to SIMS analysis, the sample was cleaned in an ultrasonicbath following a three-stage cleaning process (ammoniacalEDTA solution, deionized water, and methanol) and a conduc-tive gold layer of 50 nm thickness was applied to the samplesurface. Uranium-Th disequilibrium dating and quantificationof selected trace elements (including rare earth elements, REE;Table S1 in the ESM) were carried out by SIMS using a large-geometry CAMECA 1280-HR ion microprobe. A mass-filtered 16O− primary ion beam was accelerated at −13 kV todeliver a probe current of ~60 nA at the sample surface. Thediameter of the primary beam was 30–40 μm, and secondaryions were extracted at +10 kV with an energy bandpass of50 eV. The oxygen-flooding technique (sample chamber pres-sure ~ 1.5 × 10−5 Pa) was used to increase the production ratesof secondary ThO+ and UO+ ions (Schuhmacher et al. 1994).Secondary ions were detected by Faraday cup (FC; for specieswith measured intensities >106 counts/s) and axial electronmultiplier (EM; for intensities
Quantification of Sc, Nb, and Ta required separate analyt-ical protocols with very high mass resolution (M/ΔM=~20,000) because the sole or predominant stable isotopes ofthese elements show isobaric interferences by hydrides andmono- or polyatomic ions: 45Sc (90Zr2+), 93Nb (92ZrH),181Ta (90Zr91Zr). Niobium was counted in static multi-collection using an axial EM with 90Zr2+ as a reference masson an FC in the C position, with the magnetic field regulated athigh mass resolution through a nuclear magnetic resonance(NMR) probe. By contrast, Sc and Ta were detected by theaxial EM in peak-hopping mode with reference masses 90Zr2+
and 91Zr for Sc measured on EM and FC2, respectively, and90Zr2 for Ta measured on the axial EM. For quantification oftrace element concentrations, zircon 91500 (Wiedenbeck et al.1995, 2004) was used as primary reference for standardizationof Sc, Nb, and Ta, and Madagascan Green zircon (MAD-559;Coble et al. 2018) served as a secondary reference to assessanalytical precision (Table S2 in the ESM). For trace elementquantification, Zr abundances were deduced from thestochiometric composition of zircon. Anomalies for Ce andEu were calculated from chondrite-normalized values as Ce/Ce* and Eu/Eu* with * marking the theoretically expectedabundances from the geometric means of adjacent REE(e.g., Kato et al. 2006).
Oxygen isotopic compositions were analysed by SIMS fol-lowing procedures in Schmitt et al. (2017). AS3 referencezircon (δ18O = +5.34‰; Trail et al. 2007) was used to correctfor instrumental mass fractionation. Data for 91,500 referencezircon (+9.63 ± 0.12‰, 1 standard error of n = 10 replicates)placed on the same mount adjacent to the unknowns agreewith the nominal value of +9.86‰ (Wiedenbeck et al. 2004)indicating that this correction is reliable. Two spots wereplaced on each crystal, and the averages of both analysis arereported per crystal in Table S1 of the ESM.
Hafnium isotopic compositions were determined as singlespots on 19 zircon crystals (Table S1 in the ESM) using LA-ICP-MS as described in Gerdes and Zeh (2006, 2009).Accuracy and reproducibilitywas checked by repeated analysesof reference zircon GJ-1 and Temora for which 176Hf/177Hfaverages of 0.282666 (n = 14) and 0.282008 (n = 20) were ob-tained in the same session during which Vesuvius zircon wasanalysed; these values closely agree with published data(Woodhead and Hergt 2005; Gerdes and Zeh 2006).
Comparative Raman microspectroscopy spectra of Vesuviuszircon and inclusions were obtained after cleaning the mountsurface to remove all conductive coatings. A Horiba JobinYvon LabRAM HR800 Raman spectrometer with a 633 nmlaser source and an 1800 groves/mm grating, and a WITecAlpha 300R Raman microscope featuring a 532 nm lasersource and a UHTS300S spectrometer with a 1200 groves/
mm grating were initially employed because comparison be-tween spectra generated with different laser wavelengths allowsthe identification of potential spectral artefacts (e.g.,photoluminescence). Spectral resolutions for the two systemswere 0.8 cm−1 and 2.6 cm−1, respectively. For Ramanmapping,a 50× objective with a numerical aperture of 0.75 was usedcorresponding to a nominal lateral resolution of ~0.9 μm forthe 532 nm laser source. Laser power on the sample surface was10 mW for the WITec instrument using the proprietaryTruePower readout. The obtained Raman spectra werecorrected for cosmic ray interference and background; bandfitting used a Voigt algorithm to display FWHM values.Wavenumber calibration was performed using a built-in Ar-Hg lamp which was also used to determine spectral resolution.Gaussian fitting of the 577 nm emission line yielded a full widthat half maximum (FWHM) value of 2.4 cm−1. A value of2.6 cm−1 was used as the instrument profile function (IPF) tocorrect bands for spectral broadening using eq. 5b from Váczi(2014). The ~1007 cm−1 ν3(SiO4) Raman band of high-puritysynthetic zircon (Guillong et al. 2015) yielded a FWHM of1.9 cm−1 on the Jobin Yvon LabRAM HR800 (IPF =0.8 cm−1) at 633 nm and an identical value for the WITecAlpha 300R in agreement with published data (Nasdala et al.2008a, 2008b). Effective alpha self-radiation doses were calcu-lated for Vesuvius zircon using measured U and Th concentra-tions, the crystallization age obtained by U/Th isochron datingand the equation by Holland and Gottfried (1955).
Optical absorption spectroscopy
Optical absorption spectroscopy in the ultraviolet-visible tonear-infrared (UV-VIS-NIR) wavelength range was carriedout using a J&MTIDASUV-VIS-NIR spectrometer equippedwith CCD/InGaAs detectors and 10× UV-transparent objec-tive lenses. Light sources include a Hg vapor lamp and axenon lamp, which generated minor spectral artefacts at656 nm, 904–1247 nm, and 1384 nm in the optical absorptionspectra. Each randomly sectioned sample was measured withpolarized light at its two extinction positions in cross polarizedlight. Light intensity without sample was tuned to 70–85% ofdetector saturation by adjusting the counting time (145 ms forthe UV and visible ranges, 190 ms for the NIR range), and100 cycles were measured at each position to improve thesignal-to-noise ratio.
Microtexture, chemical and isotopic composition, andage
Vesuvius zircon shows oscillatory zoning in all studied grains,with additional sector zoning present in a few crystals, that is
26 Y. Sun et al.
visible both in BSE and CL images (Fig. 2 b–c; 4 a–c). Micro-inclusions of mineral phases occur concentrated in vesicle-richdomains where the zircon host is low in BSE intensity. Thesezones are characterized by low trace element abundances(based on SEM-EDS analysis) and are aligned along crystallo-graphically oriented growth zones or primary cracks (Fig. 2 b–c), which were also imaged in three-dimensions for a selectedzircon (Animation S1 in the ESM). The inclusions are of eitherisometric or irregular, elongated shape and exhibit a large var-iation in grain sizes (Fig. 2 b–d). While a few larger inclusionsup to ~60 μm in diameter are present, most inclusion dimen-sions are in the micro- to nanometer range (~2.5 μm –
colouration in heat-treated Ratanakiri zircon are highly depen-dent on the individual composition of the grains, as samplesfrom the same experimental runs attained different shades ofblue. Regardless, the intensity of the blue colouration gener-ally increased with lower fO2 and increasing heating duration.The most intense blue colour in Ratanakiri zircon wasachieved by heating at 1000 °C in 100% CO atmosphere for>15 h. Under oxidizing conditions, untreated dark-brown andpreviously blue Ratanakiri zircon faded to light brown or or-ange after being heated to 1000 °C for 24 h in ambient air,consistent with observations in Zeug et al. (2018).
After heating under oxidizing conditions Vesuvius zirconcrystals developed a muddy yellow-brown colour (Fig. 7 a).Heat-treatment under reducing conditions did not induce sig-nificantly changes of colouration in Vesuvius blue zircon (Fig.7 b–c). The yellow-brown colouration generated by heatingunder oxidizing conditions ismost prominent in inclusion-richzircon domains (Fig.7 d–h), whereas transparent zircon zonesdevoid of microscopically visible inclusions still retain a paleblue colouration (Fig. 7 a).
UV radiation had no visible effect (neither short-wave norlong-wave) on the colouration of Vesuvius zircon. By con-trast, the blue colour of heat-treated Ratanakiri zircon turnedinto a slightly brownish hue when irradiated by long-wave UVlight (365 nm).
Optical absorption spectroscopy
Optical absorption spectra obtained from Ratanakiri zircon (aheat-treated blue gem crystal) show a strongly polarized ab-sorption band at ~640 nm that is typical for blue zircon fromRatanakiri (Zeug et al. 2018) and elsewhere (Fig. 8 a–b). Theoptical absorption spectra of untreated and heat-treated (bothoxidizing and reducing conditions) Vesuvius zircon, however,are characterized by the presence of multiple sharp lines thatare typical for zircon rich in actinides and lanthanides (e.g., U,Th, Ce) (Nasdala et al. 2003) and a gentle increase in absor-bance towards shorter wavelengths (Fig. 8 c–d; Table S4–5 inthe ESM). All major sharp bands can be attributed with U4+-bands (e.g., at 654.0 nm, 691.2 nm, and 1115.5 nm) detectedin U-rich zircon, e.g. Mogok green zircon (Fig. 8 c; http://minerals.gps.caltech.edu/FILES/Visible/zircon/Index.html;last accessed 10.03.2020). Heated and natural Vesuvius zirconsamples share the same spectral characteristics and showminor differences in total intensities, with higher intensitiesobserved for the sample heated under oxidizing conditionsand decreased absorption for the sample treated underreduced conditions.
Vesuvius blue zircon shows a FWHM for the ν3(SiO4) Ramanband at ~1007 cm−1 ranging from ~3 to ~9 cm−1 (Fig. 4 and
Fig. 4 Overview BSE (a) and CL (b) images of natural Vesuvius zircon(grain 19) showing oscillatory zonation cross-cut by intergrowth of lowBSE intensity zircon domains dotted with abundant inclusions showinghigh BSE intensities. Ramanmicrospectroscopy map (c) generated with a532 nm laser using lateral step widths of 1 μm. Colour scale shows thefull width at half maximum (FWHM) of the ~1007 cm−1 ν3(SiO4) bandafter correction for spectral broadening. Note the reduction in FWHM inirregular, inclusion-rich zones (especially in the left part of the exposedcrystal), as well as in growth domains with high BSE intensities. Crossesare fiduciary marks
28 Y. Sun et al.
Fig. S4–6 in the ESM). A broad photoluminescence signalcausing elevated backgrounds at ~1007 cm−1 is present insome spectra generated with 633 nm excitation (Figs. S4and 5 in the ESM at points 1 and 4), but not in the spectraobtained with 532 nm excitation. Raman microspectroscopymapping reveals that homogeneous zircon domains high inBSE intensity generally have broader (and possibly split)bands compared to domains low in BSE intensity (Fig. 4 c).Mapping also reveals that the original oscillatory zonation isoverprinted by irregular and often cross-cutting zones wherethe FWHM of the ~1007 cm−1 band is reduced relative to theoriginal domain; these zones are typically inclusion-richwhere zircon shows low and inclusions high BSE intensities(Fig. 4). Variations in FWHM for the ~1007 cm−1 band alsocorrelate with a minor shift to lower Raman-shift values e.g.from 1008 cm−1 (low BSE intensity) to 1004 cm−1 (high BSEintensity; Fig. S4–S6 in ESM). Bands are narrowest (~3 cm−1)in domains with large inclusions where zircon has low BSEintensity (point 1 in Fig. 4) and in those with low BSE inten-sities and no inclusions (point 2). High-brightness BSE do-mains without inclusions have intermediate FWHM values(point 3), whereas the widest bands (~9 cm−1) were detectedin zones where zircon has high BSE brightness, and inclusionsare scarce or absent (point 4; see also example spectra forthese domains in Fig. S5 in the ESM).
Using Th and U abundances of homogeneous zirconshowing high BSE intensities and the U-Th isochron age,an effective self-radiation dose of 2.20 × 1011 α/mg was
calculated for Vesuvius zircon. Because of the wt% levelTh and U abundances of Vesuvius zircon, these low effec-tive α-doses are owed primarily to minor exposure times toself-radiation due to their very young crystallization age.This calculated dose value is well below the minimumself-radiation dose of 0.1 × 1018 α/g (Zhang et al. 2000,Nasdala et al. 2004) required to induce minute, spectroscop-ically detectable structural damage in zircon. Thereforeband broadening in Vesuvius zircon is not due to accumu-lated radiation damage (e.g., Nasdala et al. 1998).
As the only naturally occurring blue zircon known, syenite-hosted zircon from the Avellino eruption of Vesuvius is a veryunusual material whose origins and causes of colour deserveattention. Geochronology and O-Hf isotopic data are consis-tent with crystallization of zircon from magmas that wereconsanguineous to the host phonolite. Textural evidence ofinterstitial zircon growth along with the unusual enrichmentin LREE imply late-stage crystallization in highly evolvedresidual melts in a largely solidified part of the pre-eruptivemagma reservoir. Oxygen isotopes are consistent withsubsolidus crystallization at conditions significantly belowphonolite eruption temperatures of ~800 °C (Barberi et al.1981; Balcone-Boissard et al. 2012). In this regard,Vesuvius blue zircon is genetically similar to syenite-hosted
Fig. 5 Uranium-Th isochrondiagram for Vesuvius blue zircon.All uncertainties plotted andstated as 1σ. The plot combines21 spot analyses on 20 differentcrystals where homogeneous,inclusion-free domains werepreferentially targeted
29Natural blue zircon from Vesuvius
zircon from other alkalinemagma systems (e.g., Eifel; Schmittet al. 2017).
Disparate behaviour under long-wave UV, strongly di-vergent trace element compositions, and prominent differ-ences in optical absorption spectra, suggest that thecolouring mechanism for natural Vesuvius zircon must bedifferent from that of heat-treated Ratanakiri zircon.Because the blue colouration of natural Vesuvius zirconremained stable after UV irradiation and heating, electronor hole defects can be ruled out as causes for its colour(e.g., Kempe et al. 2016). Trace elements do not seem to
significantly contribute to the colouration of Vesuvius bluezircon either. Vanadium, which is responsible for the
Fig. 6 Darkfield (DF) and plane-polarised transmitted light (PPL) photomicrographs of synthetic cryolite glass (a–b), natural Vesuvius blue zircon (c–d),and blue Ratanakiri zircon, which was heat-treated under reducing conditions (e–f)
Fig. 7 Vesuvius zircon crystals after heating under (a) oxidizing and (b)reducing conditions. Areas which have remained bluish after heat-treatment under oxidizing conditions are marked by dashed lines in (a).Polished thick sections of natural (c) and (d) Vesuvius zircon heat-treatedunder oxidizing conditions in reflected light (RL) on white background;e–f) the same crystals in PPL on a dark background and g–h) as BSEimages. Arrows are drawn as fiduciary markers indicating the orientationof the crystals
30 Y. Sun et al.
31Natural blue zircon from Vesuvius
colour of synthetic blue zircon pigment (e.g., Demiray et al.1970; Waal et al. 1996), is present in concentrations belowSIMS limits of detection (
quartz indicate that a relatively small inclusion density (0.5–1.7 particles 5 particles of
und U abundances are low as indicated by homogeneouslylow BSE intensities and comparatively narrow Raman bands(e.g., point 2, Fig. 4. Our preferred model for the formation ofVesuvius blue zircon (Fig. 9) also explains why it is rare innature: it requires high abundances of Th and/or U to exsolvetiny inclusions, but at the same time these actinide-rich zirconcrystals are highly vulnerable to internal radiation damagewhich produces electron traps and the corresponding brown-ish red to nearly black (“malacon”) colour of zircon (Rossman1981).
The emergence of a yellowish-brown colouration in inclu-sion-rich, re-equilibrated zones of Vesuvius zircon after heattreatment under oxidizing conditions remains ambiguous.Scanning electron microscopy and Raman microspectroscopyfailed to detect chemical or structural changes in either hostzircon or inclusion phases, and inclusions appeared un-changed in frequency, size, and shape after heating. Opticalspectroscopy of the brown-coloured domains was not success-ful due to their poor transparency, resulting in insufficienttransmission rates. The most reasonable redox-sensitive chro-mophore would be U4+/U5+, as a contribution of Fe2+/Fe3+ isunlikely based on the low Fe abundances in zircon and mostinclusion phases (e.g., thorianite, thorite) as indicated bySIMS analysis and optical absorption spectroscopy (see spec-trum obtained on transparent domains in heated Vesuvius zir-con; Table S6 of the ESM). Oxidation of Fe-bearingpyrochlore group minerals, however, is possible as they con-tain up to 0.5 wt% Fe as detected by standardless EDS anal-yses. Oxidation of Fe2+ and possibly U4+ in inclusion phasesis thus tentatively invoked as the cause for the browncolouration of heat-treated Vesuvius zircon.
Vesuvius blue zircon is an unusual mineral which combineshighly elevated concentrations of Th (up to 5.9 wt%) and U(up to 1.8 wt%) with low radiation damage due to its veryyoung (3.41 ± 0.59 ka) crystallization age. Partialdissolution-reprecipitation of originally high-Th and high-Uzircon occurred along fractures or internal growth zones priorto eruption, causing exsolution of abundant micro- tonanometre scale mineral inclusions. Rayleigh and/orMie scat-tering of light on the smallest of these inclusions is a feasiblemechanism to explain the blue colour of Vesuvius zircon.Vesuvius zircon is thus not a natural occurring analogue forheat-treated blue zircon gemstones, which are low in actinidesand lack corresponding mineral inclusions that could causescattering (Zeug et al. 2018).
Acknowledgements We are grateful to Ilona Fin and Oliver Wienand(Heidelberg University) for the preparation of epoxy mounts, thin andthick sections. Alexander Varychev and Jan Schmitt (Heidelberg
University) are thanked for their assistance with the scanning electronmicroscope and the Raman microscope, and Axel Gerdes (GoetheUniversity Frankfurt) for measuring Hf isotope data. Shuang-Qing Li(Heidelberg University) is thanked for providing sample material ofRatanakiri zircon. Proof reading by Janet Harvey improved the English.Constructive comments by F. Lin Sutherland and two anonymous journalreviewers, and diligent editorial handling by Lutz Nasdala are gratefullyacknowledged.
Funding Open Access funding enabled and organized by Projekt DEAL.
Open Access This article is licensed under a Creative CommonsAttribution 4.0 International License, which permits use, sharing,adaptation, distribution and reproduction in any medium or format, aslong as you give appropriate credit to the original author(s) and thesource, provide a link to the Creative Commons licence, and indicate ifchanges weremade. The images or other third party material in this articleare included in the article's Creative Commons licence, unless indicatedotherwise in a credit line to the material. If material is not included in thearticle's Creative Commons licence and your intended use is notpermitted by statutory regulation or exceeds the permitted use, you willneed to obtain permission directly from the copyright holder. To view acopy of this licence, visit http://creativecommons.org/licenses/by/4.0/.
Ayuso RA, De Vivo B, Rolandi G, Seal RR II, Paone A (1998)Geochemical and isotopic (Nd–Pb–Sr–O) variations bearing onthe genesis of volcanic rocks from Vesuvius, Italy. J VolcanolGeotherm Res 82:53–78
Balcone-Boissard H, Boudon G, Ucciani G, Villemant B, Cioni R,Civetta L, Orsi G (2012) Magma degassing and eruption dynamicsof the Avellino pumice Plinian eruption of Somma-Vesuvius (Italy).Comparison with the Pompeii eruption. Earth Planet Sci Lett 331:257–268
Barberi F, Bizouard H, Clocchiatti R, Metrich N, Santacroce R, Sbrana A(1981) The Somma-Vesuvius magma chamber: a petrological andvolcanological approach. Bull Volcanol 44:295–315
Cioni R, Santacroce R, Sbrana A (1999) Pyroclastic deposits as a guidefor reconstructing the multi-stage evolution of the Somma-Vesuviuscaldera. Bull Volcanol 61:207–222
Coble MA, Vazquez JA, Barth AP, Wooden J, Burns D, Kylander-ClarkA, Jackson S, Vennari CE (2018) Trace element characterisation ofMAD-559 zircon reference material for ion microprobe analysis.Geostand Geoanal Res 42:481–497
Deer WA, Howie RA, Zussman J (1982) Rock-forming minerals:orthosilicates, volume 1A. Geological Society of London
Demiray T, Nath DK, Hummel FA (1970) Zircon-vanadium blue pig-ment. J Am Ceram Soc 53:1–4
Di Renzo V, Di Vito MA, Arienzo I, Carandente A, Civetta L, D'antonioM, Giordano F, Orsi G, Tonarini S (2007) Magmatic history ofSomma–Vesuvius on the basis of new geochemical and isotopicdata from a deep borehole (Camaldoli della Torre). J Petrol 48:753–784
DrakeMJ,Weill DF (1972) New rare earth element standards for electronmicroprobe analysis. Chem Geol 10:179–181
Faulkner MJ, Shigley JE (1989) Zircon from the harts range, northernterritory, Australia. Gems Gemol 25:207–215
34 Y. Sun et al.
Feng T, Lang C, Pasek MA (2019) The origin of blue coloration in afulgurite from Marquette, Michigan. Lithos 342:288–294
Fritsch E, Rossman GR (1988) An update on color in gems. Part 3: colorscaused by band gaps and physical phenomena. Gems Gemol 24(2):81–102
Fulignati P, Marianelli P, Santacroce R, Sbrana A (2004) Probing theVesuvius magma chamber–host rock interface through xenoliths.Geol Mag 141:417–428
Gasperini D, Blichert-Toft J, Bosch D, Del Moro A, Macera P, AlbaredeF (2002) Upwelling of deep mantle material through a plate win-dow: evidence from the geochemistry of Italian basaltic volcanics. JGeophys Res Solid Earth 107:7–19
Geisler T, Schaltegger U, Tomaschek F (2007) Re-equilibration of zirconin aqueous fluids and melts. Elements 3:43–50
Gerdes A, Zeh A (2006) Combined U–Pb and Hf isotope LA-(MC-) ICP-MS analyses of detrital zircons: comparison with SHRIMP and newconstraints for the provenance and age of an Armoricanmetasediment in Central Germany. Earth Planet Sci Lett 249:47–61
Gerdes A, Zeh A (2009) Zircon formation versus zircon alteration—newinsights from combined U–Pb and Lu–Hf in-situ LA-ICP-MS anal-yses, and consequences for the interpretation of Archean zircon fromthe central zone of the Limpopo Belt. Chem Geol 261:230–243
Guillong M, Schmitt AK, Bachmann O (2015) Comment on “zircon U–Th–Pb dating using LA-ICP-MS: simultaneous U–Pb and U–Thdating on 0.1 ma Toya Tephra, Japan” by Hisatoshi Ito. JVolcanol Geotherm Res 296:101–103
Holland HD, Gottfried D (1955) The effect of nuclear radiation on thestructure of zircon. Acta Cryst 8:291–300
Huong LTT, Vuong BS, Thuyet NTM, Nguyen NK, Satitkune S,Wanthanachaisaeng B, Hofmeister W, Häger T, Hauzenberger C(2016) Geology, gemmological properties and preliminary heattreatment of gem-quality zircon from the central highlands ofVietnam. J Gemmol 35:308–318
Kato Y, Yamaguchi KE, Ohmoto H (2006) Rare earth elements inPrecambrian banded iron formations: secular changes of Ce andEu anomalies and evolution of atmospheric oxygen. In: Kesler SE,Ohmoto H (eds) Evolution of early Earth’s atmosphere, hydro-sphere, and biosphere - constraints from ore deposits, vol 198.Geol Soc Am Mem, pp 269–289
Kempe U, Trinkler M, Pöppl A, Himcinschi C (2016) Coloration ofnatural zircon. Can Mineral 54(3):635–660
Kostov I (1973) Zircon morphology as a crystallogenetic indicator. KristTech 8:11–19
Krzemnicki MS, Butini F, Butini E, De Carolis E (2019) Gemmologicalanalysis of a Roman sapphire intaglio and its possible origin. JGemmol 36:710–724
Marini L, Chiappini V, Cioni R, Cortecci G, Dinelli E, Principe C, FerraraG (1998) Effect of degassing on sulfur contents and δ34S values inSomma-Vesuvius magmas. Bull Volcanol 60:187–194
Medenbach O, Shannon RD (1997) Refractive indices and optical dis-persion of 103 synthetic and mineral oxides and silicates measuredby a small-prism technique. J Optical Soc Am B 14:3299–3318
Linde N, Ricci T, Shakas A, Berrino G (2017) The 3-D structure of theSomme-Vesuvius volcanic complex (Italy) inferred from new andhistoric gravity data. Sci Rep 7:1–10
Lockwood DJ (2016) Rayleigh and Mie scattering. In: Encyclopedia ofcolor science and technology. Springer, New York, pp 1–12
McDonough WF, Sun SS (1995) The composition of the earth. ChemGeol 120:223–253
Nasdala L, Pidgeon RT, Wolf D, Irmer G (1998) Metamictization and U-Pb isotopic discordance in single zircons: a combined Raman mi-croprobe and SHRIMP ion probe study. Mineral Petrol 62:1–27
Nasdala L, Zhang M, Kempe U, Panczer G, Gaft M, Andrut M, Plötze M(2003) Spectroscopic methods applied to zircon. In: Hanchar JW,Hoskin PWO (eds) Zircon. Rev Mineral Geochem, vol 53. MinerSoc Am, Washington DC, pp 427–467
Nasdala L, Reiners PW, Garver JI, Kennedy AK, Stern RA, Balan E,Wirth R (2004) Incomplete retention of radiation damage in zirconfrom Sri Lanka. Am Mineral 89:219–231
Nasdala L, Hofmeister W, Norberg N, Martinson JM, Corfu F, Dörr W,Kamo SL, Kennedy AK, Kronz A, Reiners PW, Frei D, Kosler J,Wan Y, Götze J, Häger T, Kröner A, Valley JW (2008a) ZirconM257- a homogeneous natural reference material for the ion micro-probe U-Pb analysis of zircon. Geostand Geoanal Res 32:247–265
Nasdala L, Miletich R, Ruschel K, Váczi T (2008b) Raman study ofradiation-damaged zircon under hydrostatic compression. PhysChem of Minerals 35(10):597–602
Paces JB, Miller JD Jr (1993) Precise U-Pb ages of Duluth complex andrelated mafic intrusions, northeastern Minnesota: Geochronologicalinsights to physical, petrogenetic, paleomagnetic, andtectonomagmatic processes associated with the 1.1 Ga midcontinentrift system. J Geophys Res Solid Earth 98:13997–14013
Pearce NJ, PerkinsWT, Westgate JA, Gorton MP, Jackson SE, Neal CR,Chenery SP (1997) A compilation of new and published major andtrace element data for NIST SRM 610 and NIST SRM 612 glassreference materials. Geostand Newslett 21(1):115–144
Pelto CR (1956) A study of chalcedony. Am J Sci 254(1):32–50Piilonen PC, Sutherland FL, Danišík M, Poirier G, Valley JW, Rowe R
(2018) Zircon xenocrysts from Cenozoic alkaline basalts of theRatanakiri Volcanic Province (Cambodia), Southeast Asia —traceelement geochemistry, O-Hf isotopic composition, U-Pb and (U-Th)/he geochronology—revelations into the underlying lithosphericmantle. Minerals 8:556
Qin T, Wu F, Wu Z, Huang F (2016) First-principles calculations ofequilibrium fractionation of O and Si isotopes in quartz, albite, an-orthite, and zircon. Contrib Mineral Petrol 171:91
Renfro ND (2016) Reversible color modification of blue zircon by long-wave ultraviolet radiation. Gems Gemol 52:256–251
Ryde JW, Cooper BS (1931) The scattering of light by turbid media – partII. Proc Royal Soc London Series A 131:464–475
Rossman GR (1981) Color in gems: the new technologies. Gems Gemol17:60–71
Rossman GR (2014) Optical spectroscopy. In: Henderson GS, NeuvilleDR, Downs RT (eds) Spectroscopic methods in mineralogy andmaterials sciences. Rev Mineral Geochem, vol 78. Miner Soc Am,Chantilly, pp 371–398
Rupasinghe MS, Senaratne A (1986) A treatment procedure for improv-ing colour and quality of zircons. J Gemm 20:168–170
Russo M, Punzo I (2004) I Minerali del Somma-Vesuvio. AssociazioneMicromineralogica Italiana, Cremona, pp 1–320
Santacroce R, Cioni R, Marianelli P, Sbrana A, Sulpizio R, Zanchetta G,Donahue DJ, Joron JL (2008) Age and whole rock-glass composi-tions of proximal pyroclastics from the major explosive eruptions ofSomma-Vesuvius: a review as a tool for distal tephrostratigraphy. JVolcanol Geotherm Res 177:1–18
Satitkune S, Wanthanachaisaeng B, Won-in K, Wongkokau W,Chantararat P, Leelawattanasuk T, Wathanakul P (2013) Heat treat-ment of zircon samples from Kanchanaburi, Thailand andRatanakiri, Cambodia. In: Henn U, Zwaan H, Fritsch E (eds)Proceedings of the 33rd international Gemmological conference.Hanoi, Vietnam, pp 158–160
SchmitzMD, Bowring SA, Ireland TR (2003) Evaluation of Duluth com-plex anorthositic series (AS3) zircon as a U-Pb geochronologicalstandard: new high-precision isotope dilution thermal ionizationmass spectrometry results. Geochim Cosmochim Acta 67:3665–3672
Schmitt AK, Klitzke M, Gerdes A, Schäfer C (2017) Zircon hafnium–oxygen isotope and trace element petrochronology of intraplate vol-canic rocks from the Eifel (Germany) and implications for mantleversus crustal origins of zircon megacrysts. J Petrol 58:1841–1870
Schuhmacher M, de Chambost E, McKeegan KD, Harrison TM, MigeonH (1994) In situ U/Pb dating of zircon with the CAMECA ims 1270.
35Natural blue zircon from Vesuvius
In: Benninghoven A, Nihei Y, Shimizu R, Werner HW (eds)Secondary ion mass spectrometry SIMS IX. Wiley, Chichester, pp919–922
Seifert W, Rhede D, Thomas R, Förster HJ, Lucassen F, Dulski P, WirthR (2011) Distinctive properties of rock-forming blue quartz: infer-ences from amulti-analytical study of submicronmineral inclusions.Mineral Mag 75:2519–2534
Sevink J, van Bergen MJ, van der Plicht J, Feiken H, Anastasia C,Huizinga A (2011) Robust date for the bronze age Avellino eruption(Somma-Vesuvius): 3945±10 calBP (1995±10 calBC). Quat SciRev 30:1035–1046
Shao T, Xia Y, Ding X, Cai Y, Song M (2019) Zircon saturation interrestrial basaltic melts and its geological implications. SolidEarth Sci 4:27–42
Sulpizio R, Cioni R, Di Vito MA, Mele D, Bonasia R, Dellino P (2010a)The Pomici di Avellino eruption of Somma-Vesuvius (3.9 ka BP).Part I: stratigraphy, compositional variability and eruptive dynam-ics. Bull Volcanol 72:539–558
Sulpizio R, Bonasia R, Dellino P, Mele D, Di Vito MA, La Volpe L(2010b) The Pomici di Avellino eruption of Somma–Vesuvius(3.9 ka BP). Part II: sedimentology and physical volcanology ofpyroclastic density current deposits. Bull Volcanol 72:559–577
Trail D, Mojzsis SJ, Harrison TM, Schmitt AK, Watson EB, Young ED(2007) Constraints on hadean zircon protoliths from oxygen iso-topes, Ti-thermometry, and rare earth elements. GeochemGeophys Geosystems 8(6):Q06014. https://doi.org/10.1029/2006GC001449
Troch J, Ellis BS, Schmitt AK, Bouvier AS, Bachmann O (2018) Thedark side of zircon: textural, age, oxygen isotopic and trace elementevidence of fluid saturation in the subvolcanic reservoir of the IslandPark-Mount Jackson rhyolite, Yellowstone (USA). Contrib MineralPetrol 173:54
Uvarova YA, Sokolova E, Hawthorne FC, Agakhanov AA, Pautov LA(2004) The crystal structure of arapovite, U4+(Ca, Na)2(K1–x□x)[Si8O20], x≈ 0.5, a new mineral of the steacyite group fromthe Dara-i-Pioz moraine, Tien-Shan mountains, Tajikistan. CanMineral 42:1005–1011
Váczi T (2014) A new, simple approximation for the deconvolution ofinstrumental broadening in spectroscopic band profiles. ApplSpectrosc 68(11):1274–1278
Waal DD, Heyns AM, Pretorius G, Clark RJ (1996) Raman spectroscopicinvestigations of ZrSiO4: V
4+, the blue zircon vanadium pigment. JRaman Spectrosc 27:657–662
Wehrmeister U, Häger T (2006) Edelsteine erkennen: Eigenschaften undBehandlung. Rühle-Diebener, Stuttgart
Wiedenbeck M, Alle P, Corfu F, Griffin WL, Meier M, Oberli F, vonQuadt A, SpiegelW (1995) Three natural zircon standards for U-Th-Pb, Lu-Hf, trace element and REE analyses. Geostand Newslett 19:1–23
Wiedenbeck M, Hanchar JM, Peck WH, Sylvester P, Valley J,Whitehouse M, Kronz A, Morishita Y, Nasdala L, Fiebig J,Franchi I, Girard JP, Greenwood RC, Hinton R, Kita N, MasonPRD, Norman M, Ogasawara M, Piccoli PM, Rhede D, Satoh H,Schulz-Dobrick B, Skår O, Spicuzza MJ, Terada K, Tindle A,Togashi S, Vennemann T, Xie Q, Zheng YF (2004) Further charac-terisation of the 91500 zircon crystal. Geostand Geoanal Res 28:9–39
Wittwer A, Nasdala L, Wanthanachaisaeng B, Bunnag N, Škoda R,Balmer WA, Giester G, Zeug M (2013) Mineralogical characterisa-tion of gem zircon fromRatanakiri, Cambodia. In: Nasdala L, GötzeJ, Hanchar JM (eds) Proceedings of the CORALS-2013: conferenceon Raman and luminescence spectroscopy in the earth sciences.Austria, Vienna, pp 115–116
Woodhead JD, Hergt JM (2005) A preliminary appraisal of seven naturalzircon reference materials for in situ Hf isotope determination.Geostandards Geoanal Res 29:183–195
YuanW, Bao Z, Dong J, Guo Z, Deng J (2007) Zircon and apatite fissiontrack analyses on mineralization ages and tectonic activities ofTuwu-Yandong porphyry copper deposit in northern Xinjiang,China. Sci China Ser D 50:1787–1795
Zeug M, Nasdala L, Wanthanachaisaeng B, Balmer WA, Corfu F,Wildner M (2018) Blue zircon from Ratanakiri, Cambodia. JGemmol 36:112–132
Zhang M, Salje EKH, Farnan I, Graeme-Barber A, Daniel P, Ewing RC,Clark AM, Lennox H (2000) Metamictization of zircon: Ramanspectroscopic study. J Phys Condens Mat 12:1915–1925
Zolensky ME, Sylvester PJ, Paces JB (1988) Origin and significance ofblue coloration in quartz from llano rhyolite (llanite), north-centralLlano County, Texas. Am Mineral 73:313–323
Zolensky ME, Koeberl C (1991) Why are blue zhamanshinites blue?Liquid immiscibility in an impact melt. Geochim CosmochimActa 55:1483–1486
Publisher’s note Springer Nature remains neutral with regard to jurisdic-tional claims in published maps and institutional affiliations.
36 Y. Sun et al.
Natural blue zircon from VesuviusAbstractIntroductionGeological settingMaterials and methodsSample material and thin-section petrographySample preparationHeating and UV irradiation experimentsOptical microscopyScanning electron microscopy (SEM) and microtomography (micro-CT)Secondary ionization mass spectrometry (SIMS) and laser ablation inductively coupled plasma mass spectrometry (LA-ICP-MS) analysisRaman microspectroscopyOptical absorption spectroscopy
ResultsMicrotexture, chemical and isotopic composition, and ageColour in optical microscopyColour change under heating and irradiationOptical absorption spectroscopyRaman microspectroscopy